Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

# Synthesis, characterization and application of organoclays for adsorptive desulfurization of fuel oil

## Abstract

The present study encompasses the application of cost effective, organo-modified bentonite material for efficient desulfurization of model oil and real fuel. For the adsorptive desulfurization of oil, dibenzothiophene (DBT) was used as model compound. Various experimental parameters (time, temperature, adsorbent-amount and DBT concentration) were thoroughly investigated. The synthesized material was characterized via X-ray diffraction (XRD), X-ray Fluorescence (XRF), Scanning electron microscopy (SEM), Energy dispersive x-ray (EDX), Thermogravimetric analysis (TGA) and Fourier transform infrared spectroscopy (FT-IR). The modification exhibits the increase in interlayer spacing of clay as confirmed from XRD and modified material shows interesting morphology as compared to unmodified bentonite. The results showed that > 90% of DBT removal was achieved under optimized conditions for B-BTC, B-BTB and B-DSS and > 80% for B-BEHA, for model fuel oil which are greater than unmodified clay (< 45%). Additionally, the findings from desulfurization of real fuel oil declare that 96.76% and 95.83% removal efficiency was achieved for kerosene and diesel oil respectively, at optimized conditions and fuel properties follow ASTM specifications. The obtained findings well fitted with thermodynamic, isothermal (Langmuir) with adsorption capacity (70.8 (B-BTC), 66 (B-BTB), 61.2 (B-DSS) and 55.2 (B-BEHA) in mg/g) and pseudo-second-order kinetics. In thermodynamic studies, negative sign ($$\Delta G^\circ )$$ specifies the spontaneity whereas, $$\left(\Delta H^\circ \right)$$ endothermic and positive sign $$(\Delta S^\circ )$$ show randomness after DBT adsorption onto organoclay.

## Introduction

Demand for the utilization of more eco-friendly fuels and their production is increasing due to the implementation of legislation requiring strict regulation of green-house gas emissions. Many countries are currently enforcing a strict control of sulfur content in liquid fuels to ultralow levels, making the production of deep desulfurization processes an important research objective1,2,3. Among the main industrial processes for the removal of sulfur from liquid fuels, the most important is referred as adsorptive desulfurization (ADS) and operates with microporous and mesoporous materials4,5,6.

As the stringent sulfur content has emerged, desulfurization of fuel has received massive attention of the world. Thiols, sulfides and disulfides can be efficiently removed using conventional adsorbents7. Various important features of adsorptive desulfurization (ADS) which have grasped attention as an alternative technology are high efficiency, moderate operation conditions and its economical rates. Similar technique is photocatalytic oxidative desulfurization (ODS) in which sulfur compounds are converted to SO4–2, sulfoxides and sulfones under photo-oxidation8. These polarized compounds can be separated from non-polar oils into extractants i.e., water, acetonitrile or ionic liquids (ILs). Numerous studies have been conducted for desulfurization of fuel oils by combining UV irradiation and liquid–liquid extraction. The center of their research (adsorptive and oxidative) lies on product identification and the effect of sulfur removal9.

Clay (low-cost and eco-friendly) is a naturally available adsorbent that has been used for the removal of dyes, heavy metals, organic pollutants, mycotoxins, sulfur content etc. form decades24,25,26. Its effectiveness is because of its layered structure that bears strong affinity regarding cations and anions and has exchangeable ions that play vital role in adsorption. Thus, it works as host material for the adsorbents with an increased surface area as well as it has significant applications in synthesis of biodiesel27,28. However, the adsorption capacity of raw clay is not as good as compared to synthetically modified clay. Once the clay surface is modified with surfactant based organic molecule, its adsorption capacity could be enhanced by leaps and bounds. For the past two decades removal of organic contaminants using modified solid material has gained much attention29,30. The clay was modified with organic molecules to form micelle-like structures on its surface that had the capability to solubilize organic pollutant such as DBT.

We herein report the removal of DBT desulfurization by a low-cost adsorbent i.e., organoclay. But hydrophilicity of interlayer surface restricts the adsorption capacity of clay for organic targets. So, benzyl tri-n-butyl ammonium bromide (BTB), Dioctyl sodium sulfosuccinate (DSS), benzethonium chloride (BTC) and Bis (2-ethylhexyl) amine (BEHA) based modified clay was observed to have improved hydrophobicity to interact strongly with the organic matter providing efficient adsorption and first time used for the removal of DBT from model fuel oil and real fuel oil. In addition, the unmodified and modified clay was characterized via FT-IR, XRF, XRD, SEM, EDX and TGA to investigate the composition of material. Adsorption studies reveal the desulfurization of mg/L level of DBT in model fuel and real fuel oil. To further investigate the adsorption capacity of the clay, adsorption kinetics (pseudo first order, pseudo second order and intraparticle diffusion model) and isotherms (Langmuir, Freundlich and Temkin model) were also studied and efficacy was monitored at different optimized conditions.

## Materials and methods

### Materials

Sodium Bentonite (Al2H2Na2O13Si4, LOT: 10195902) pristine clay (2:1) (BT) and modification reagent; benzyl tri-n-butyl ammonium bromide (BTB), Dioctyl sodium sulfosuccinate (DSS), benzethonium chloride (BTC) and Bis (2-ethylhexyl) amine (BEHA) were obtained from Alfa Aesar Co., Germany and used without any modification. The targeted adsorbate Dibenzothiophene (DBT) was obtained from Sigma Aldrich Co., used for adsorption study.

### Material synthesis

Modified bentonite (B-BTB, B-DSS, B-BTC and B-BEHA) were synthesized via modification regent by dispersing the 1 g of bentonite (BT) in 50 mL of water through sonication (for the dispersion of clay particles into water) for 30 min at room temperature, reported previously24,25,26. The pH (4) was maintained by using 0.5 M HCl to make clear suspension of above solution. 0.3 g of modification reagent (BTB, DSS, BTC or BEHA) was dissolved in 50 mL of water and added into above suspension and refluxed stirring was carried out for 6 h at 120 °C. The synthesized material was subjected to filtration, dried at 120 °C in oven and grounds via pestle mortar.

Adsorption of Dibenzothiophene (DBT) on to unmodified clay (BT) and synthesized organoclay (B-BTB, B-DSS, B-BTC and B-BEHA) was conducted with different concentrations of DBT in isooctane. The optimization studies were performed with 30 mL of 1000 mg/L DBT solution with 0.5 g of organoclay. Centrifugation and filtration were used for the separation of adsorbent and adsorbate (DBT solution). The calibration curve was obtained by UV/Vis spectrophotometer (Shimadzu UV1700 Japan) and PETRA X-Ray Sulfur Analyzer, ASTM D-4294) was used to analyze the residual amount of DBT. The percentage efficiency (S%) and adsorption capacity (qe) at equilibrium for adsorption of DBT were determined by following Eqs. (1) and (2)24,31:

$$Sorption\, Efficiency\, \left( {S\% } \right) = \frac{{\left( {Ci - Ce} \right)}}{Ci} \times 100$$
(1)
$$qe = \frac{{\left( {Ci - Ce} \right) \times V}}{m}$$
(2)

Here, Ce and Ci = equilibrium and initial DBT concentrations (mg/L), qe = adsorption capacity of synthesized organoclay (mg/g), V = solution volume, m = mass of organoclay by weight (g).

### Instrumentation

The unmodified bentonite (BT) and synthesized materials (B-BTB, B-DSS, B-BTC and B-BEHA) were characterized via XRD; Powder X-ray diffractometer (PXRD) of Cu-Kα = 1.54 Å in the range of (2θ = 5–70°) with scan rate (2°, 2θ/min), SEM; Scanning electron microscopy (NOVA Nano), EDX; Energy dispersive X-ray spectroscopy for elemental composition and FTIR; Fourier transform infrared spectroscopy, ATR/IRTRACER-100 with resolution rate of (15 scan and 1 cm-1) in the range of (4000–400 cm-1). In addition, X-ray fluorescence spectrometer (XRF, Bruker S8) was used to determine the chemical composition. TGA study was also investigated for the quantification of organic moieties in the layers of clay by heating in the range of (40–800 °C), inert atmosphere (Helium, 30 mL/min) with heating rate (30 °C/min). Moreover, PETRA-X-ray Fluorescence (XRF) sulfur analyzer (ASTM D-4294) used to analyze the residual amount of sulfur compounds.

## Results and discussion

### Material characterization

#### FT-IR

In order to affirm the presence of functional groups at the adsorbent surface, FT-IR spectral analysis of both modified and unmodified material (BT) was carried out (range 4000–400 cm-1) as shown in Fig. 1. The 3480 cm-1 band that appears only in unmodified material due to interlayer water molecules i.e., corresponds to –OH stretching vibrations. The band in the range of 1470–1350 cm-1 and 2950–2800 cm-1 appears only for modified material is characteristic and corresponds to C–H bending and stretching vibrations, thus absent in unmodified material. The sp3 C–H stretch for B-BEHA is (2876 cm-1), sp2 C–H stretch for B-BEHA (2964 cm-1), CH3 bending vibration for B-BEHA is (1379 cm-1), CH2 bending vibration for B-BEHA (1481 cm-1). These stretching and bending vibrations are confirms the functional groups of the adsorbent surface that has been modified and are similar to the FT-IR described previously26,32,33.

#### XRD and XRF

Powder X-ray Diffraction studies was carried out to investigate the peak shifting towards lower 2θ value in modified clay that increase the interlayered d-spacing of clay material26,32,34. The Fig. 2 shows the pXRD pattern of pristine clay (Fig. 2a) along with the modified clays, most of the peaks in modified pXRD pattern is same as the pristine bentonite clay as confirmed by the Joint Committee on Powder Diffraction Standards card (JCPDS No. 00-003-0015) except one peak that is observed at 2θ = 9.23° with basal d-spacing 0.96 nm in pristine clay. If there is a shifting of this peak observed towards lower 2θ values, it shows the increase in interlayer spacing due to intercalation of organic molecule26,32,34. The modified bentonite shows the peak shifting of B-DSS (2θ = 6.44°, 1.37 nm), B-BTC (2θ = 6.97°, 1.26 nm), B-BTB (2θ = 6.79°, 1.30 nm), B-BEHA (2θ = 7.61°, 1.15 nm) (Fig. 2b–e), which are similar to previous reported studies26,32,34.

Chemical composition of pristine clay (unmodified) as determined via XRF study was found to be: CaO = 5.01%, Na2O = 2.1%, Al2O3 = 23.9%, MgO = 2.9%, SiO2 = 55.1% and K2O = 3.48%. This data indicates that; Na, Mg, K and Ca are prime exchangeable cations24.

#### SEM

The micrographs of unmodified and modified bentonite material were observed via Scanning electron microscopy (SEM Nano NOVA) to confirm the presence of organic moieties into galleries of clay particles and changes in morphology after modification. It seems that the pristine clay exhibits the grasps foliated with massive curved like plates and tightly held as shown in Figure which become foamy, fluffy and more porous after modification as given in Fig. 335,36. Moreover, in modified clay there are bigger porous aggregates that provide more residence to adsorbate and have extra available bonding sites for adsorption of DBT. Additionally, regarding as quantification of elemental analysis in modified clay material via EDX, more carbon content was observed in organoclay than carbon content in unmodified bentonite material because when we loaded the organic molecules (DSS, BTC, BTB and BEHA) into the galleries of clay, the amount of carbon increases in modified materials. The observed carbon content: B-DSS (18.7 wt. %), B-BTC (23.4 wt. %), B-BTB (21.3 wt. %) and B-BEHA (16.9 wt. %) which is absent in unmodified bentonite. The observed components of bentonite clay are present naturally expect carbon content which is observed after modification. The presence of carbon loading indicates the effective synthesis of modified materials (B-DSS, B-BTC, B-BTB and B-BEHA) that results in increase the adsorption capacity of DBT molecules owing to increase in d-spacing of clay galleries after modification as confirmed from XRD.

#### TGA

The stability of modified and unmodified material was determined by analyzing weight loss over a range of temperature (i.e., 40–840 °C) under inert atmosphere via TGA as given in Fig. 4. Transitions of unmodified material during thermal degradation were at low temperature the surface adsorbed water that volatilize (below 140 °C), at high temperature (450–600 °C) due to –OH group de-hydroxylation of water occurred. The four regions of thermal degradation in modified materials occurred as following; the physically adsorbed gaseous substances and water evolved (below 150 °C), the organic specie (BTC, BTB, DSS and BEHA) decomposed (between 200 and 450 °C), structural water loss caused de-hydroxylation (450–600 °C) and the carbonaceous organic products evolved (between 600 and 700 °C)24,26. The increased adsorption capacity of modified materials has successfully been demonstrated by the comparison of modified and unmodified material.

#### Effect of contact time and temperature on DBT adsorption

The effect of contact time on the removal of DBT onto BT, B-BTC, B-DSS, B-BTB and B-BEHA was observed at various time intervals by keeping the adsorbent dose 0.5 g, volume = 30 mL and DBT concentration 1000 mg/L as constant. The adsorption of DBT onto organoclay increases with increase of contact time. At the beginning the adsorption process is fast and gradually slows down in order to attain stability. The maximum adsorption occurs at 60 min. Hence 60 min is marked for higher efficiency of adsorption process as shown in Fig. 5a17. Furthermore, to find out the optimum temperature the desulfurization of DBT was carried out by varying temperature in the range of 25–45 $$^\circ{\rm C}$$ and other parameters were remained constant. The results depict that the adsorption efficiency has direct relation with temperature (Fig. 5b). At higher temperature, Dibenzothiophene (DBT) is more mobile due to reducing the viscosity as well as higher temperature lead the widens of adsorbent pores to some extent and results in decrease the activation energy19.

The effect of adsorbent dosage (organoclay) and unmodified clay on the desulfurization of DBT was investigated by varying the amount of dose (0.25–1.25 g) and the DBT concentration of 1000 mg/L, time = 60 min and volume = 30 mL at 45 $$^\circ{\rm C}$$ as shown in Fig. 5c. The results declared that adsorption efficiency (%) is directly proportional to adsorbent dose and inversely proportional to adsorption capacity. This decrease in adsorption capacity of DBT with increased adsorbent dose is because of larger number of adsorption sites (organic moieties) as well as mass of adsorbent dose has indirect relation with adsorption capacity (qe) as shown in Eq. (2). Hence at lesser adsorbent dosage the adsorption capacity is maximum as observed19. The adsorbent (B-BTC) has high percentage of DBT removal than B-BTB, B-DSS and B-BEHA due to presence of two phenyl groups that are more active functional groups and enhances the adsorption proves due to its pi–pi interaction with DBT molecule.

#### Effect of DBT concentration

Adsorption capacity of organoclays is altered by varying the concentration of DBT. Five different concentrations (500–2000 mg/L) were used for the investigation of DBT concentration effects on adsorption of DBT keeping remaining parameters as constant (adsorbent dose = 0.5 g, volume = 30 mL, time = 60 min and at 45 $$^\circ{\rm C}$$). In general, adsorption capacity increases with increasing concentration of DBT until the availability of the adsorbent. Yet the efficiency is affected, as it limits the available sites (fixed amount of adsorbent) for the DBT molecules (at high levels) but can still work with reduced efficiency. DBT removal and adsorption capacity of organoclay illustrate opposite fashion, which can be elucidated as binding sites of organoclay are fixed. When less concentration of DBT is available the faster will be the adsorption and the percent removal will be high, as higher numbers of binding sites are present on the organoclay37. More the presence of binding sites on organoclay, lesser the concentration of the DBT molecules, the most efficient will be the adsorption process as shown in Fig. 5d.

#### Kinetic study

For understanding the mechanism of adsorption process, kinetic study is of prime importance. During adsorption of DBT on to adsorbent (BT, B-BTC, B-DSS, B-BTB and B-BEHA), undergoes various processes from bulk solution onto organoclay surface (adsorbent). For adsorption mechanism, pseudo-first order and pseudo-second order kinetic models were applied. Pseudo-first order is valid for adsorption of adsorbate from aqueous solution (physisorption). The integral form of Pseudo-first order kinetic model is represented as Eq. (3)38:

$$\log \left( {q_{e} - qt} \right) = \log \left( {q_{e} } \right) - \frac{{K_{1} }}{2.303}t$$
(3)

where qt is amount of DBT adsorbed at time, qe is at equilibrium the amount of DBT adsorbed, K1 pseudo-first order constant. Rate constant, intercept and slope were calculated from linear plot (log (qe − qt) vs. time).

The pseudo-second order kinetic model is based on “the rate involves forces for sharing or exchanging of electrons between adsorbate and adsorbent (chemisorption)”. Pseudo-second order kinetic model is represented as Eq. (4)38:

$$\frac{{dq_{t} }}{dt} = k_{2} (q_{e} - q_{t} )^{2}$$
(4)

Rearranging Eq. (4) by integrating within boundary conditions at qt = 0 to t = 0 and qt = qt to t = t, (5):

$$\frac{t}{{q_{t} }} = \frac{1}{{k_{2} q_{e}^{2} }} + \frac{t}{{q_{e} }}$$
(5)

where $$k_{2}$$ pseudo-second order constant, Slope $$\left( {\frac{t}{{q_{t} }}} \right)$$ and intercept $$\left( {\frac{1}{{k_{2} qe^{2} }}} \right)$$ were used for calculating $$k_{2}$$ and qe.

The optimized situations for the studies contain 0.5 g of organoclay, 1000 mg/L of DBT concentration with range of time scale as given in Table 1. The regression coefficient ($${R}^{2}$$) of pseudo-second order is better than pseudo-first order for the organoclay. So, the data indicates the chemisorption mechanism (pseudo second order kinetics) for the adsorption of specific DBT onto modified materials B-DSS, B-BTB, B-BTC and B-BEHA as shown in Fig. 6 and physisorption mechanism (pseudo first order kinetics) followed onto unmodified bentonite material (BT). In addition, the calculated adsorption capacity (qm) for pseudo second order kinetics is greater than experimental (qm) for the adsorption of DBT via organoclay.

To study the mass transfer rate comparison for the adsorption of DBT, the intraparticle diffusion model (Fickian-diffusion) model was also applied and it represents as Eq. (6)38:

$${\text{qt}} = K_{p} t^{1/2} + C$$
(6)

where C is intercept (determined from qt vs t1/2 plot) and kp is rate constant (mgg-1 min-1/2) as values are given in Table 1. This Fickian-diffusion model is studied to evaluate the rate controlling step (t = 10–100 min) and the plot is not linear as well as R2 (0.881, 0.899, 0.936 and 0.931 for B-BTC, B-BTB, B-DSS and B-BEHA respectively) which is quite lower than pseudo second order kinetics. The obtained findings declared that this model is not fitted well as compared to pseudo second order kinetic model, but it also indicate that the DBT adsorption onto organoclay may also be followed by intraparticle diffusion model.

Equilibrium adsorption was analyzed by different isotherm models. The amount of adsorbed DBT and its concentration in solution were shown by Langmuir and Freundlich isotherm. Langmuir model shows the adsorption of DBT molecules on to adsorbent surface, happens on homogenous monolayer surface deprived of any interaction with neighboring adsorbed molecules. Langmuir isotherm equation is given as Eq. (7)24:

$$\frac{{C_{e} }}{{q_{e} }} = \frac{{C_{e} }}{{q_{m} }} + \frac{1}{{K_{L} q_{m} }}$$
(7)

where $$K_{L}$$ is Langmuir adsorption equilibrium constant associated with free energy and $$q_{m}$$ is maximum adsorption capacity of organoclay. The adsorption isotherm is plotted by $$\frac{{C_{e} }}{{q_{e} }} vs C_{e}$$, and data should give straight line, which is appropriate for this model where, slope is $$\frac{1}{{q_{m} }}$$ and intercept $$\frac{1}{{K_{L} q_{m} }}$$ . Regarding as Langmuir Isotherm model; there is no interaction among the adsorbed molecules. The distinctiveness of Langmuir isotherm model was expressed via RL parameter (dimensionless constant) that is expressed in Eq. (8):

$$R_{L} = \frac{1}{1 + KL \cdot Co}$$
(8)

RL parameter point out the nature of DBT adsorption onto organoclay either; irreversible (RL = 0), unfavorable (RL > 1), favorable (0 < RL < 1) and linear (RL = 1).

Freundlich adsorption isotherm is for multilayer formation that occurs due to heterogeneous adsorption. Freundlich adsorption isotherm equation is given as Eq. (9)37:

$$\ln q_{e} = \ln K_{F} + \frac{1}{{n_{F} }}\ln C_{e}$$
(9)

where $$q_{e}$$ is the amount of adsorbate, adsorbed on the surface of adsorbent at equilibrium, $$C_{e}$$ is equilibrium adsorbate concentration, $$K_{F}$$ is Freundlich constant and $$\frac{1}{{n_{F} }}$$ is heterogeneity factor. For favorable adsorption $$n_{F}$$ is large than 1. The values for slope $$\frac{1}{{n_{F} }}$$ and intercept $$\ln K_{F}$$ were obtained from linear plot of $${\text{ ln}}q_{e} vs\ln C_{e}$$.

Table 2 and Fig. 7 include the experimental results at optimized conditions (0.5 g adsorbent dose and 1000 mg/L of DBT concentration) of isothermal models, though the regression coefficient ($${R}^{2}$$) of Langmuir model is best for DBT removal, which indicates the monolayer adsorption of sulfur molecules on the surface of organoclay. Moreover, the calculated value of qm = 33.78 (BT), 70.8 (B-BTC), 66 (B-BTB), 61.2 (B-DSS) and 55.2 (B-BEHA) in (mg/g) by using Langmuir model is very close to the experimental observed qm = 28.26 (BT), 71.43 (B-BTC), 66.66 (B-BTB), 62.50 (B-DSS) and 57.14 (B-BEHA) mg/g which clearly indicated the monolayer adsorption phenomenon. The RL value is lesser than 1 which indicating the favorability of DBT adsorption onto both unmodified and organoclay. Moreover, the order of adsorptive desulfurization is B-BTC > B-BTB > B-DSS > B-BEHA > BT.

To examine the adsorbate-adsorbent interaction for the adsorption of DBT onto unmodified and modified bentonite, we further applied a Temkin model. The general representing of Temkin model is given in Eq. (10)19:

$$q_{e} = BlnC_{e} + BlnA$$
(10)

where A (Temkin constant (L/g) that is related to adsorbate–adsorbate interaction), B (Heat of adsorption in J/mol) and qe (equilibrium adsorbed amount (mg/g)). The heat of adsorption and regression coefficient (R2) is given in Table 2 which indicates that the Temkin model is not well fitted as compared to Langmuir isotherm model.

#### Thermodynamic studies of DBT adsorption

To understand the effect of different temperatures for the removal of DBT from fuel oil via organoclay, various thermodynamic paramters i.e., standard entropy, standard enthalpy and standard Gibbs Free energy has been thoroughly studied. The above procedure was conducted with 30 mL of (1000 mg/L) initail (DBT) solution at various temperatures (298.5, 303.5, 318.5, and 333.5 K) along with 0.5 g (modified clay) for an hour. Using following Eq. (11) Gibbs Free energy was calculated19:

$$\Delta G^\circ = - RT\ln K_{c}$$
(11)

Moreover, Standard entropy was calculated using Vant’s Hoff Eq. (12) by plotting InKc vs 1/T and standard enthalpy was calculated using Eq. (13)39:

$$lnK_{c} = - \frac{\Delta H^\circ }{{RT}} + \frac{\Delta S^\circ }{R}$$
(12)
$$\Delta G^\circ = \Delta H^\circ - T\Delta S^\circ$$
(13)

where Kc = Organoclay retention ability to hold the (DBT) which is calculated through Eq. (14):

$$K_{c} = \frac{{q_{e} }}{{C_{e} }}$$
(14)

Here Ce is the adsorbed Organoclay equilibrium concentration while qe is the (DBT) equilibrium concentration.

The van der wall forces exist between organoclay (B-BTC, B-DSS, B-BTB and B-BEHA) and DBT molecules were reduced by triggers the weak interaction at low temperature and at high temperature optimum adsorption was observed, thus it gives neagtive values of $$\Delta G^\circ$$. However , positive value of enthalpy was justified the endothermic nature of adsorption. Besides this during the adsorption of (DBT), the positive values of $$\Delta S^\circ$$ indicates the irregularity in randomness onto synthesized oragnoclay as given in Table 3.

The adsorptive desulfurization of commercially available fuel samples (Kerosene and Diesel) was also investigated via modified bentonite material (B-BTC) under optimized conditions (time = 60 min, adsorbent = 0.5 g, volume = 30 mL and temperature = 45 $$^\circ {\text{C}}$$) and before desulfurization the total sulfur content in kerosene and diesel oil was found to be 2848 mg/L and 4468 mg/L respectively. The concentration is too high to be removed under the optimized conditions, therefore the dilution of the sample was carried out with iso-octane to get the sulfur content in the range of 1200 mg/L. To quantify the amount of sulfur components PETRA X-Ray Fluorescence Spectrophotometer (XRF) (ppm, ASTM D-4294) was used. Moreover, other fuel properties such as specific gravity, water content and distillation were also conducted via Hydrometer (g/mL @ 15.6 $$^\circ {\text{C}}$$, ASTM D-1298), Water content tester (China PT-D4006-8929A) (vol. %, ASTM D-4006) and Distillation tester (PMD 110, PAC) (ASTM D-86). The findings declared that 96.76% and 95.83% removal efficiency was achieved for kerosene and diesel oil respectively and the other fuel characteristics before and after ADS are given in Table 4. Moreover, the unmodified bentonite was also tested for the desulfurization of fuel oil but due to lower interlayer spacing of clay the results was not efficient as compared to modified bentonite material. Upon modification the increase in d-spacing and development of interesting morphology (porous and fluffy) results in the increase in adsorption capacity.

#### Compariosn with other reported methods

Due to limited available data for the DBT desulfurization via organo-clay based modified materials, we can not make comparison for the adsorption efficiency effectively. Moreover, we have compared adsorpton capacity (mg/g) for the DBT removal with other modified adsorbents as given in Table 5. It can be seen that the proposed method shows better adsorption capacity than the reported methods.

## References

1. Saha, B., Vedachalam, S. & Dalai, A. K. Review on recent advances in adsorptive desulfurization. Fuel Processing Technology, 106685 (2020).

2. Zhang, P., Mao, X. & Yang, B. Mechanistic study on adsorption desulfurization using modified graphene. Ind. Eng. Chem. Res. 58, 10589–10598 (2019).

3. Zhang, P., Mao, X., Mi, R., Wang, L. & Yang, B. Mesoporous silica encapsulated phosphotungstic acid catalysts for alkylation desulfurization of gasoline. Catal. Lett. 151, 95–106. https://doi.org/10.1007/s10562-020-03288-8 (2021).

4. Dehghan, R. & Anbia, M. Zeolites for adsorptive desulfurization from fuels: a review. Fuel Process. Technol. 167, 99–116 (2017).

5. Luo, J. et al. Design of lewis acid centers in bundlelike boron nitride for boosting adsorptive desulfurization performance. Ind. Eng. Chem. Res. 58, 13303–13312. https://doi.org/10.1021/acs.iecr.9b01745 (2019).

6. Luo, J. et al. High-performance adsorptive desulfurization by ternary hybrid boron carbon nitride aerogel. AIChE J. 67, e17280. https://doi.org/10.1002/aic.17280 (2021).

7. Lee, K. X. & Valla, J. A. Adsorptive desulfurization of liquid hydrocarbons using zeolite-based sorbents: a comprehensive review. React. Chem. Eng. 4, 1357–1386 (2019).

8. Babich, I. & Moulijn, J. Science and technology of novel processes for deep desulfurization of oil refinery streams: a review. Fuel 82, 607–631 (2003).

9. Choi, A. E. S., Roces, S., Dugos, N. & Wan, M.-W. Adsorption of benzothiophene sulfone over clay mineral adsorbents in the frame of oxidative desulfurization. Fuel 205, 153–160 (2017).

10. Choi, A. E. S., Roces, S., Dugos, N., Arcega, A. & Wan, M.-W. Adsorptive removal of dibenzothiophene sulfone from fuel oil using clay material adsorbents. J. Clean. Prod. 161, 267–276 (2017).

11. Mu, L. et al. BN/ZIF-8 derived carbon hybrid materials for adsorptive desulfurization: Insights into adsorptive property and reaction kinetics. Fuel 288, 119685. https://doi.org/10.1016/j.fuel.2020.119685 (2021).

12. Abbasov, V. M., Ibrahimov, H. C., Mukhtarova, G. S., Rustamov, M. I. & Abdullayev, E. Adsorptive desulfurization of the gasoline obtained from low-pressure hydrocracking of the vacuum residue using a nickel/bentonite catalyst. Energy Fuels 31, 5840–5843 (2017).

13. Mikhail, S., Zaki, T. & Khalil, L. Desulfurization by an economically adsorption technique. Appl. Catal. A 227, 265–278 (2002).

14. Shahmirzadi, M. A. A., Hosseini, S. S., Luo, J. & Ortiz, I. Significance, evolution and recent advances in adsorption technology, materials and processes for desalination, water softening and salt removal. J. Environ. Manage. 215, 324–344 (2018).

15. Jha, D., Haider, M. B., Kumar, R., Shim, W. G. & Sivagnanam, B. M. Batch and continuous adsorptive desulfurization of model diesel fuels using graphene nanoplatelets. J. Chem. Eng. Data 65, 2120–2132 (2020).

16. Kwon, J. M. et al. Adsorptive desulfurization and denitrogenation of refinery fuels using mesoporous silica adsorbents. ChemSusChem Chem. Sustain. Energy Mater. 1, 307–309 (2008).

17. Ishaq, M. et al. Adsorptive desulfurization of model oil using untreated, acid activated and magnetite nanoparticle loaded bentonite as adsorbent. J. Saudi Chem. Soc. 21, 143–151 (2017).

18. Srivastav, A. & Srivastava, V. C. Adsorptive desulfurization by activated alumina. J. Hazard. Mater. 170, 1133–1140 (2009).

19. Ullah, S. et al. Desulfurization of model oil through adsorption over activated charcoal and bentonite clay composites. Chem. Eng. Technol. 43, 564–573 (2020).

20. Shah, S. S., Ahmad, I. & Ahmad, W. Adsorptive desulphurization study of liquid fuels using Tin (Sn) impregnated activated charcoal. J. Hazard. Mater. 304, 205–213 (2016).

21. Saleh, T. A., Sulaiman, K. O., AL-Hammadi, S. A., Dafalla, H. & Danmaliki, G. I. Adsorptive desulfurization of thiophene, benzothiophene and dibenzothiophene over activated carbon manganese oxide nanocomposite: with column system evaluation. J. Clean. Prod. 154, 401-412 (2017).

22. Li, X. et al. Synthesis, modification, and application of hollow mesoporous carbon submicrospheres for adsorptive desulfurization. Ind. Eng. Chem. Res. 57, 15020–15030 (2018).

23. Danmaliki, G. I. & Saleh, T. A. Effects of bimetallic Ce/Fe nanoparticles on the desulfurization of thiophenes using activated carbon. Chem. Eng. J. 307, 914–927 (2017).

24. Saeed, M. et al. Synthesis, characterization and applications of silylation based grafted bentonites for the removal of Sudan dyes: Isothermal, kinetic and thermodynamic studies. Microporous Mesoporous Mater. 291, 109697 (2020).

25. Wahab, N. et al. Synthesis, characterization, and applications of silk/bentonite clay composite for heavy metal removal from aqueous solution. Front. Chem. 7, 654 (2019).

26. Saeed, M. et al. Green and eco-friendly removal of mycotoxins with organo-bentonites; isothermal, kinetic, and thermodynamic studies. Clean: Soil, Air, Water 48, 1900427 (2020).

27. Munir, M. et al. Sustainable production of bioenergy from novel non-edible seed oil (Prunus cerasoides) using bimetallic impregnated montmorillonite clay catalyst. Renew. Sustain. Energy Rev. 109, 321–332 (2019).

28. Munir, M. et al. Production of high quality biodiesel from novel non-edible Raphnus raphanistrum L. seed oil using copper modified montmorillonite clay catalyst. Environ. Res. 193, 110398 (2021).

29. Awasthi, A., Jadhao, P. & Kumari, K. Clay nano-adsorbent: structures, applications and mechanism for water treatment. SN Appl. Sci. 1, 1–21 (2019).

30. Ali, F. D. Adsorptive desulfurization of liquid fuels using Na-bentonite adsorbents. Al-Nahrain J. Eng. Sci. 21, 248–252 (2018).

31. Morsy, A. et al. Isothermal, kinetic, and thermodynamic studies for solid-phase extraction of uranium (VI) via hydrazine-impregnated carbon-based material as efficient adsorbent. Nucl. Sci. Tech. 30, 1–11 (2019).

32. Su, J., Huang, H.-G., Jin, X.-Y., Lu, X.-Q. & Chen, Z.-L. Synthesis, characterization and kinetic of a surfactant-modified bentonite used to remove As (III) and As (V) from aqueous solution. J. Hazard. Mater. 185, 63–70 (2011).

33. Zhang, Y. et al. Adsorption of mixed cationic-nonionic surfactant and its effect on bentonite structure. J. Environ. Sci. 24, 1525–1532 (2012).

34. Ullah, H. et al. Adsorption Kinetics of Malachite green and Methylene blue from aqueous solutions using surfactant-modified Organoclays. Acta Chim. Slov. 64, 449–460 (2017).

35. Ikhtiyarova, G., Özcan, A., Gök, Ö. & Özcan, A. Characterization of natural-and organo-bentonite by XRD, SEM, FT-IR and thermal analysis techniques and its adsorption behaviour in aqueous solutions. Clay Miner. 47, 31–44 (2012).

36. Stepova, K. V., Maquarrie, D. J. & Krip, I. M. Modified bentonites as adsorbents of hydrogen sulfide gases. Appl. Clay Sci. 42, 625–628 (2009).

37. Sadare, O. O. & Daramola, M. O. Adsorptive desulfurization of dibenzothiophene (DBT) in model petroleum distillate using functionalized carbon nanotubes. Environ. Sci. Pollut. Res. 26, 32746–32758 (2019).

38. Jha, D. et al. Enhanced adsorptive desulfurization using Mongolian anthracite-based activated carbon. ACS Omega 4, 20844–20853 (2019).

39. Tariq, S. et al. Green and eco-friendly adsorption of dyes with organoclay: isothermal, kinetic and thermodynamic studies. Toxin Rev. 1–10 (2021).

40. Chen, T.-C., Agripa, M. L., Lu, M.-C. & Dalida, M. L. P. Adsorption of sulfur compounds from diesel with ion-impregnated activated carbons. Energy Fuels 30, 3870–3878 (2016).

41. Lu, M.-C., Agripa, M. L., Wan, M.-W. & Dalida, M. L. P. Removal of oxidized sulfur compounds using different types of activated carbon, aluminum oxide, and chitosan-coated bentonite. Desalin. Water Treat. 52, 873–879 (2014).

42. Jha, D. et al. Adsorptive removal of dibenzothiophene from diesel fuel using microwave synthesized carbon nanomaterials. Fuel 244, 132–139 (2019).

43. Saleh, T. A. & Danmaliki, G. I. Adsorptive desulfurization of dibenzothiophene from fuels by rubber tyres-derived carbons: kinetics and isotherms evaluation. Process Saf. Environ. Prot. 102, 9–19 (2016).

44. Cheng, J., Jin, S., Zhang, R., Shao, X. & Jin, M. Enhanced adsorption selectivity of dibenzothiophene on ordered mesoporous carbon-silica nanocomposites via copper modification. Microporous Mesoporous Mater. 212, 137–145 (2015).

45. Haji, S. & Erkey, C. Removal of dibenzothiophene from model diesel by adsorption on carbon aerogels for fuel cell applications. Ind. Eng. Chem. Res. 42, 6933–6937 (2003).

46. Nejad, N. F., Shams, E., Amini, M. & Bennett, J. Synthesis of magnetic mesoporous carbon and its application for adsorption of dibenzothiophene. Fuel Process. Technol. 106, 376–384 (2013).

## Acknowledgements

The authors are grateful to Deanship of Scientific Research, Qassim University, Saudi Arabia for funding the publication of this project.

## Author information

Authors

### Contributions

M.S. and A.R: Formal analysis, M.S. and A. I.: Writing – original draft, : H.F., and H.H.: Investigation, Methodology, M.I.Z. and A.A.: Writing – review and editing, A.W.: Conceptualization, Supervision. A.W. and A.A.: correspondence for publication. All authors reviewed the manuscript.

### Corresponding authors

Correspondence to Aiyeshah Alhodaib or Amir Waseem.

## Ethics declarations

### Competing interests

The authors declare no competing interests.

### Publisher's note

Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

Saeed, M., Riaz, A., Intisar, A. et al. Synthesis, characterization and application of organoclays for adsorptive desulfurization of fuel oil. Sci Rep 12, 7362 (2022). https://doi.org/10.1038/s41598-022-11054-6

• Accepted:

• Published:

• DOI: https://doi.org/10.1038/s41598-022-11054-6